DOI: 10.17188/1700873
title: Materials Data on Li3Mn2(P2O7)2 by Materials Project

description: Li3Mn2(P2O7)2 crystallizes in the triclinic P1 space group. The structure is three-dimensional. there are twelve inequivalent Li1+ sites. In the first Li1+ site, Li1+ is bonded in a 5-coordinate geometry to five O2- atoms. There are a spread of Li–O bond distances ranging from 1.99–2.28 Å. In the second Li1+ site, Li1+ is bonded to four O2- atoms to form distorted LiO4 tetrahedra that share corners with four PO4 tetrahedra, a cornercorner with one MnO5 trigonal bipyramid, and an edgeedge with one MnO6 octahedra. There are a spread of Li–O bond distances ranging from 1.94–2.08 Å. In the third Li1+ site, Li1+ is bonded to four O2- atoms to form distorted LiO4 tetrahedra that share corners with four PO4 tetrahedra, a cornercorner with one MnO5 trigonal bipyramid, and an edgeedge with one LiO4 tetrahedra. There are a spread of Li–O bond distances ranging from 1.93–1.97 Å. In the fourth Li1+ site, Li1+ is bonded in a 5-coordinate geometry to five O2- atoms. There are a spread of Li–O bond distances ranging from 1.95–2.62 Å. In the fifth Li1+ site, Li1+ is bonded to four O2- atoms to form LiO4 tetrahedra that share corners with four PO4 tetrahedra and an edgeedge with one LiO4 tetrahedra. There are a spread of Li–O bond distances ranging from 1.82–1.97 Å. In the sixth Li1+ site, Li1+ is bonded in a distorted see-saw-like geometry to four O2- atoms. There are a spread of Li–O bond distances ranging from 1.89–2.04 Å. In the seventh Li1+ site, Li1+ is bonded in a 4-coordinate geometry to four O2- atoms. There are a spread of Li–O bond distances ranging from 1.88–2.06 Å. In the eighth Li1+ site, Li1+ is bonded to four O2- atoms to form distorted LiO4 tetrahedra that share corners with four PO4 tetrahedra, a cornercorner with one MnO5 trigonal bipyramid, and an edgeedge with one LiO4 tetrahedra. There are a spread of Li–O bond distances ranging from 1.92–1.96 Å. In the ninth Li1+ site, Li1+ is bonded in a 5-coordinate geometry to five O2- atoms. There are a spread of Li–O bond distances ranging from 1.95–2.56 Å. In the tenth Li1+ site, Li1+ is bonded to four O2- atoms to form LiO4 tetrahedra that share corners with four PO4 tetrahedra and an edgeedge with one LiO4 tetrahedra. There are a spread of Li–O bond distances ranging from 1.82–2.00 Å. In the eleventh Li1+ site, Li1+ is bonded to four O2- atoms to form distorted LiO4 tetrahedra that share corners with four PO4 tetrahedra and an edgeedge with one MnO6 octahedra. There are a spread of Li–O bond distances ranging from 1.95–2.09 Å. In the twelfth Li1+ site, Li1+ is bonded in a 5-coordinate geometry to five O2- atoms. There are a spread of Li–O bond distances ranging from 1.95–2.25 Å. There are eight inequivalent Mn+2.50+ sites. In the first Mn+2.50+ site, Mn+2.50+ is bonded to six O2- atoms to form MnO6 octahedra that share corners with six PO4 tetrahedra and an edgeedge with one MnO5 trigonal bipyramid. There are a spread of Mn–O bond distances ranging from 1.97–2.19 Å. In the second Mn+2.50+ site, Mn+2.50+ is bonded to five O2- atoms to form distorted MnO5 trigonal bipyramids that share corners with two LiO4 tetrahedra, corners with five PO4 tetrahedra, and an edgeedge with one MnO6 octahedra. There are a spread of Mn–O bond distances ranging from 2.10–2.28 Å. In the third Mn+2.50+ site, Mn+2.50+ is bonded in a 6-coordinate geometry to six O2- atoms. There are a spread of Mn–O bond distances ranging from 2.07–2.76 Å. In the fourth Mn+2.50+ site, Mn+2.50+ is bonded to six O2- atoms to form MnO6 octahedra that share corners with six PO4 tetrahedra and an edgeedge with one LiO4 tetrahedra. There are a spread of Mn–O bond distances ranging from 1.96–2.22 Å. In the fifth Mn+2.50+ site, Mn+2.50+ is bonded to six O2- atoms to form MnO6 octahedra that share corners with six PO4 tetrahedra, an edgeedge with one LiO4 tetrahedra, and an edgeedge with one MnO5 trigonal bipyramid. There are a spread of Mn–O bond distances ranging from 1.94–2.22 Å. In the sixth Mn+2.50+ site, Mn+2.50+ is bonded to five O2- atoms to form distorted MnO5 trigonal bipyramids that share a cornercorner with one LiO4 tetrahedra, corners with five PO4 tetrahedra, and an edgeedge with one MnO6 octahedra. There are a spread of Mn–O bond distances ranging from 2.11–2.32 Å. In the seventh Mn+2.50+ site, Mn+2.50+ is bonded in a 5-coordinate geometry to five O2- atoms. There are a spread of Mn–O bond distances ranging from 2.08–2.32 Å. In the eighth Mn+2.50+ site, Mn+2.50+ is bonded to six O2- atoms to form MnO6 octahedra that share corners with six PO4 tetrahedra. There are a spread of Mn–O bond distances ranging from 1.99–2.17 Å. There are sixteen inequivalent P5+ sites. In the first P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share a cornercorner with one MnO6 octahedra, a cornercorner with one LiO4 tetrahedra, a cornercorner with one PO4 tetrahedra, and corners with two MnO5 trigonal bipyramids. The corner-sharing octahedral tilt angles are 48°. There are a spread of P–O bond distances ranging from 1.52–1.59 Å. In the second P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share a cornercorner with one MnO6 octahedra, a cornercorner with one PO4 tetrahedra, and corners with two LiO4 tetrahedra. The corner-sharing octahedral tilt angles are 34°. There are a spread of P–O bond distances ranging from 1.49–1.64 Å. In the third P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share a cornercorner with one MnO6 octahedra, a cornercorner with one PO4 tetrahedra, and corners with two LiO4 tetrahedra. The corner-sharing octahedral tilt angles are 55°. There are a spread of P–O bond distances ranging from 1.51–1.62 Å. In the fourth P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share corners with three MnO6 octahedra, a cornercorner with one LiO4 tetrahedra, and a cornercorner with one PO4 tetrahedra. The corner-sharing octahedra tilt angles range from 31–52°. There are a spread of P–O bond distances ranging from 1.52–1.61 Å. In the fifth P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share corners with three MnO6 octahedra, a cornercorner with one LiO4 tetrahedra, and a cornercorner with one PO4 tetrahedra. The corner-sharing octahedra tilt angles range from 36–49°. There are a spread of P–O bond distances ranging from 1.53–1.60 Å. In the sixth P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share a cornercorner with one MnO6 octahedra, a cornercorner with one PO4 tetrahedra, corners with three LiO4 tetrahedra, and corners with two MnO5 trigonal bipyramids. The corner-sharing octahedral tilt angles are 54°. There are a spread of P–O bond distances ranging from 1.51–1.63 Å. In the seventh P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share a cornercorner with one MnO6 octahedra, a cornercorner with one PO4 tetrahedra, and corners with two MnO5 trigonal bipyramids. The corner-sharing octahedral tilt angles are 50°. There are a spread of P–O bond distances ranging from 1.50–1.60 Å. In the eighth P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share a cornercorner with one MnO6 octahedra, a cornercorner with one PO4 tetrahedra, corners with two LiO4 tetrahedra, and a cornercorner with one MnO5 trigonal bipyramid. The corner-sharing octahedral tilt angles are 37°. There are a spread of P–O bond distances ranging from 1.51–1.61 Å. In the ninth P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share a cornercorner with one MnO6 octahedra, a cornercorner with one PO4 tetrahedra, and corners with two LiO4 tetrahedra. The corner-sharing octahedral tilt angles are 35°. There are a spread of P–O bond distances ranging from 1.49–1.62 Å. In the tenth P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share a cornercorner with one MnO6 octahedra and a cornercorner with one PO4 tetrahedra. The corner-sharing octahedral tilt angles are 54°. There are a spread of P–O bond distances ranging from 1.50–1.61 Å. In the eleventh P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share a cornercorner with one MnO6 octahedra, a cornercorner with one PO4 tetrahedra, and corners with three LiO4 tetrahedra. The corner-sharing octahedral tilt angles are 54°. There are a spread of P–O bond distances ranging from 1.51–1.63 Å. In the twelfth P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share corners with three MnO6 octahedra, a cornercorner with one LiO4 tetrahedra, and a cornercorner with one PO4 tetrahedra. The corner-sharing octahedra tilt angles range from 32–49°. There are a spread of P–O bond distances ranging from 1.53–1.61 Å. In the thirteenth P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share corners with three MnO6 octahedra, a cornercorner with one LiO4 tetrahedra, and a cornercorner with one PO4 tetrahedra. The corner-sharing octahedra tilt angles range from 34–52°. There are a spread of P–O bond distances ranging from 1.52–1.61 Å. In the fourteenth P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share a cornercorner with one MnO6 octahedra, a cornercorner with one PO4 tetrahedra, corners with two LiO4 tetrahedra, and corners with two MnO5 trigonal bipyramids. The corner-sharing octahedral tilt angles are 55°. There are a spread of P–O bond distances ranging from 1.51–1.62 Å. In the fifteenth P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share a cornercorner with one MnO6 octahedra, a cornercorner with one PO4 tetrahedra, corners with two LiO4 tetrahedra, and a cornercorner with one MnO5 trigonal bipyramid. The corner-sharing octahedral tilt angles are 36°. There are a spread of P–O bond distances ranging from 1.51–1.63 Å. In the sixteenth P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share a cornercorner with one MnO6 octahedra, a cornercorner with one LiO4 tetrahedra, and a cornercorner with one PO4 tetrahedra. The corner-sharing octahedral tilt angles are 51°. There are a spread of P–O bond distances ranging from 1.51–1.61 Å. There are fifty-six inequivalent O2- sites. In the first O2- site, O2- is bonded in a trigonal planar geometry to two Li1+ and one P5+ atom. In the second O2- site, O2- is bonded in a distorted trigonal planar geometry to one Li1+, one Mn+2.50+, and one P5+ atom. In the third O2- site, O2- is bonded in a distorted trigonal planar geometry to two Mn+2.50+ and one P5+ atom. In the fourth O2- site, O2- is bonded in a distorted trigonal planar geometry to one Li1+, one Mn+2.50+, and one P5+ atom. In the fifth O2- site, O2- is bonded in a distorted bent 120 degrees geometry to two P5+ atoms. In the sixth O2- site, O2- is bonded in a bent 150 degrees geometry to one Mn+2.50+ and one P5+ atom. In the seventh O2- site, O2- is bonded in a 4-coordinate geometry to two Li1+, one Mn+2.50+, and one P5+ atom. In the eighth O2- site, O2- is bonded in a distorted trigonal planar geometry to two Li1+ and one P5+ atom. In the ninth O2- site, O2- is bonded in a bent 120 degrees geometry to two P5+ atoms. In the tenth O2- site, O2- is bonded in a 3-coordinate geometry to two Li1+, one Mn+2.50+, and one P5+ atom. In the eleventh O2- site, O2- is bonded in a distorted rectangular see-saw-like geometry to one Li1+, two Mn+2.50+, and one P5+ atom. In the twelfth O2- site, O2- is bonded in a 3-coordinate geometry to one Li1+, one Mn+2.50+, and one P5+ atom. In the thirteenth O2- site, O2- is bonded in a distorted trigonal planar geometry to one Li1+, one Mn+2.50+, and one P5+ atom. In the fourteenth O2- site, O2- is bonded in a 3-coordinate geometry to one Li1+, one Mn+2.50+, and one P5+ atom. In the fifteenth O2- site, O2- is bonded in a 4-coordinate geometry to two Li1+, one Mn+2.50+, and one P5+ atom. In the sixteenth O2- site, O2- is bonded in a trigonal non-coplanar geometry to one Li1+